LMucko/crystallography-open-database huggingface dataset:
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .2, synthesized at 800 C, 1 GPa, 1 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010220
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .2, synthesized at 800 C, 1 GPa, 1 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.8 Mg0.2 O3'
_chemical_name_mineral           Otavite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.8638
_cell_length_b                   4.8638
_cell_length_c                   16.0679
_cell_formula_units_Z            6
_cell_volume                     329.186
_database_code_amcsd             0004341
_exptl_crystal_density_diffrn    4.685
_exptl_crystal_pressure_history  'synthesized at 800 C, 1 GPa, 1 h'
_exptl_crystal_thermal_history   'synthesized at 800 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Cd.8 Mg.2) C O3'
_cod_database_code               9010220
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .3, synthesized at 800 C, 1 GPa, 1 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010221
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .3, synthesized at 800 C, 1 GPa, 1 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.7 Mg0.3 O3'
_chemical_name_mineral           Otavite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.8341
_cell_length_b                   4.8341
_cell_length_c                   15.9434
_cell_formula_units_Z            6
_cell_volume                     322.658
_database_code_amcsd             0004342
_exptl_crystal_density_diffrn    4.508
_exptl_crystal_pressure_history  'synthesized at 800 C, 1 GPa, 1 h'
_exptl_crystal_thermal_history   'synthesized at 800 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Cd.7 Mg.3) C O3'
_cod_database_code               9010221
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .4, synthesized at 800 C, 1 GPa, 1 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010222
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .4, synthesized at 800 C, 1 GPa, 1 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.6 Mg0.4 O3'
_chemical_name_mineral           Otavite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.8095
_cell_length_b                   4.8095
_cell_length_c                   15.8358
_cell_formula_units_Z            6
_cell_volume                     317.227
_database_code_amcsd             0004343
_exptl_crystal_density_diffrn    4.308
_exptl_crystal_pressure_history  'synthesized at 800 C, 1 GPa, 1 h'
_exptl_crystal_thermal_history   'synthesized at 800 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Cd.6 Mg.4) C O3'
_cod_database_code               9010222
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .5, synthesized at 800 C, 1 GPa, 1 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010223
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .5, synthesized at 800 C, 1 GPa, 1 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.5 Mg0.5 O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7788
_cell_length_b                   4.7788
_cell_length_c                   15.6968
_cell_formula_units_Z            6
_cell_volume                     310.441
_database_code_amcsd             0004344
_exptl_crystal_density_diffrn    4.120
_exptl_crystal_pressure_history  'synthesized at 800 C, 1 GPa, 1 h'
_exptl_crystal_thermal_history   'synthesized at 800 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Cd.5 Mg.5) C O3'
_cod_database_code               9010223
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .6, synthesized at 800 C, 1 GPa, 1 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010224
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .6, synthesized at 800 C, 1 GPa, 1 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.4 Mg0.6 O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.7510
_cell_length_b                   4.7510
_cell_length_c                   15.5745
_cell_formula_units_Z            6
_cell_volume                     304.449
_database_code_amcsd             0004345
_exptl_crystal_density_diffrn    3.913
_exptl_crystal_pressure_history  'synthesized at 800 C, 1 GPa, 1 h'
_exptl_crystal_thermal_history   'synthesized at 800 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Cd.4 Mg.6) C O3'
_cod_database_code               9010224
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = .9, synthesized at 800 C, 1 GPa, 1 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010225
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = .9, synthesized at 800 C, 1 GPa, 1 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Cd0.1 Mg0.9 O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.6638
_cell_length_b                   4.6638
_cell_length_c                   15.1720
_cell_formula_units_Z            6
_cell_volume                     285.794
_database_code_amcsd             0004346
_exptl_crystal_density_diffrn    3.246
_exptl_crystal_pressure_history  'synthesized at 800 C, 1 GPa, 1 h'
_exptl_crystal_thermal_history   'synthesized at 800 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Cd.1 Mg.9) C O3'
_cod_database_code               9010225
Order and miscibility in the otavite - magnesite solid solution Sample: X_Mg = 1, synthesized at 800 C, 1 GPa, 1 h
Bromiley, F. A.; Boffa Ballaran, T.; Langenhorst, F.; Seifert, F.; American Mineralogist 92 (2007) 829–836; doi:10.2138/am.2007.2315

data_9010226
_publ_section_title
;
 Order and miscibility in the otavite - magnesite solid solution
 Sample: X_Mg = 1, synthesized at 800 C, 1 GPa, 1 h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              829
_journal_page_last               836
_journal_paper_doi               10.2138/am.2007.2315
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Mg O3'
_chemical_name_mineral           Magnesite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.6334
_cell_length_b                   4.6334
_cell_length_c                   15.0178
_cell_formula_units_Z            6
_cell_volume                     279.214
_database_code_amcsd             0004347
_exptl_crystal_density_diffrn    3.009
_exptl_crystal_pressure_history  'synthesized at 800 C, 1 GPa, 1 h'
_exptl_crystal_thermal_history   'synthesized at 800 C'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        'Mg C O3'
_cod_database_code               9010226
The geometric effects of VFe2+ for VMg substitution on the crystal structures of the grandidierite-ominelite series Sample: G17 Locality: Madagascar
Dzikowski, T. J.; Groat, L. A.; Grew, E. S.; American Mineralogist 92 (2007) 863–872; doi:10.2138/am.2007.2275

data_9010227
_publ_section_title
;The geometric effects of VFe2+ for VMg substitution on the crystal structures
 of the grandidierite-ominelite series Sample: G17 Locality: Madagascar
;
_journal_name_full               'American Mineralogist'
_journal_page_first              863
_journal_page_last               872
_journal_paper_doi               10.2138/am.2007.2275
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Madagascar
_chemical_formula_sum            'Al3 B Fe0.024 Mg0.976 O9 Si'
_chemical_name_mineral           Grandidierite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.3250
_cell_length_b                   10.9575
_cell_length_c                   5.7600
_cell_formula_units_Z            4
_cell_volume                     651.664
_database_code_amcsd             0004348
_exptl_crystal_density_diffrn    2.945
_cod_original_formula_sum        '(Mg.976 Fe.024) Al3 B Si O9'
_cod_database_code               9010227
The geometric effects of VFe2+ for VMg substitution on the crystal structures of the grandidierite-ominelite series Sample: G8 Locality: Long Lake, Larsemann Hills, Antarctica
Dzikowski, T. J.; Groat, L. A.; Grew, E. S.; American Mineralogist 92 (2007) 863–872; doi:10.2138/am.2007.2275

data_9010228
_publ_section_title
;The geometric effects of VFe2+ for VMg substitution on the crystal structures
 of the grandidierite-ominelite series Sample: G8 Locality: Long Lake,
 Larsemann Hills, Antarctica
;
_journal_name_full               'American Mineralogist'
_journal_page_first              863
_journal_page_last               872
_journal_paper_doi               10.2138/am.2007.2275
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        'Long Lake, Larsemann Hills, Antarctica'
_chemical_formula_sum            'Al3 B Fe0.126 Mg0.874 O9 Si'
_chemical_name_mineral           Grandidierite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.3330
_cell_length_b                   10.9858
_cell_formula_units_Z            4
_cell_length_c                   5.7667
_cell_volume                     654.614
_database_code_amcsd             0004349
_exptl_crystal_density_diffrn    2.964
_cod_original_formula_sum        '(Mg.874 Fe.126) Al3 B Si O9'
_cod_database_code               9010228
The geometric effects of VFe2+ for VMg substitution on the crystal structures of the grandidierite-ominelite series Sample: G4 Locality: Sahakondra, Ampamatoa, Madagascar
Dzikowski, T. J.; Groat, L. A.; Grew, E. S.; American Mineralogist 92 (2007) 863–872; doi:10.2138/am.2007.2275

data_9010229
_publ_section_title
;The geometric effects of VFe2+ for VMg substitution on the crystal structures
 of the grandidierite-ominelite series Sample: G4 Locality: Sahakondra,
 Ampamatoa, Madagascar
;
_journal_name_full               'American Mineralogist'
_journal_page_first              863
_journal_page_last               872
_journal_paper_doi               10.2138/am.2007.2275
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        'Sahakondra, Ampamatoa, Madagascar'
_chemical_formula_sum            'Al3 B Fe0.182 Mg0.818 O9 Si'
_chemical_name_mineral           Grandidierite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.3317
_cell_length_b                   10.9904
_cell_formula_units_Z            4
_cell_length_c                   5.7634
_cell_volume                     654.431
_database_code_amcsd             0004350
_exptl_crystal_density_diffrn    2.983
_cod_original_formula_sum        '(Mg.818 Fe.182) Al3 B Si O9'
_cod_database_code               9010229
The geometric effects of VFe2+ for VMg substitution on the crystal structures of the grandidierite-ominelite series Sample: G12 Locality: Zimbabwe
Dzikowski, T. J.; Groat, L. A.; Grew, E. S.; American Mineralogist 92 (2007) 863–872; doi:10.2138/am.2007.2275

data_9010230
_publ_section_title
;The geometric effects of VFe2+ for VMg substitution on the crystal structures
 of the grandidierite-ominelite series Sample: G12 Locality: Zimbabwe
;
_journal_name_full               'American Mineralogist'
_journal_page_first              863
_journal_page_last               872
_journal_paper_doi               10.2138/am.2007.2275
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        Zimbabwe
_chemical_formula_sum            'Al3 B Fe0.274 Mg0.726 O9 Si'
_chemical_name_mineral           Grandidierite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.3347
_cell_length_b                   11.0034
_cell_length_c                   5.7627
_cell_formula_units_Z            4
_cell_volume                     655.316
_database_code_amcsd             0004351
_exptl_crystal_density_diffrn    3.008
_cod_original_formula_sum        '(Mg.726 Fe.274) Al3 B Si O9'
_cod_database_code               9010230
The geometric effects of VFe2+ for VMg substitution on the crystal structures of the grandidierite-ominelite series Sample: G1 Locality: Karibe area, Zimbabwe
Dzikowski, T. J.; Groat, L. A.; Grew, E. S.; American Mineralogist 92 (2007) 863–872; doi:10.2138/am.2007.2275

data_9010231
_publ_section_title
;The geometric effects of VFe2+ for VMg substitution on the crystal structures
 of the grandidierite-ominelite series Sample: G1 Locality: Karibe area,
 Zimbabwe
;
_journal_name_full               'American Mineralogist'
_journal_page_first              863
_journal_page_last               872
_journal_paper_doi               10.2138/am.2007.2275
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        'Karibe area, Zimbabwe'
_chemical_formula_sum            'Al3 B Fe0.334 Mg0.666 O9 Si'
_chemical_name_mineral           Grandidierite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.3360
_cell_length_b                   11.0148
_cell_formula_units_Z            4
_cell_length_c                   5.7657
_cell_volume                     656.419
_database_code_amcsd             0004352
_exptl_crystal_density_diffrn    3.022
_cod_original_formula_sum        '(Mg.666 Fe.334) Al3 B Si O9'
_cod_database_code               9010231
The geometric effects of VFe2+ for VMg substitution on the crystal structures of the grandidierite-ominelite series Sample: G2 Locality: Andrahomana, Madagascar
Dzikowski, T. J.; Groat, L. A.; Grew, E. S.; American Mineralogist 92 (2007) 863–872; doi:10.2138/am.2007.2275

data_9010232
_publ_section_title
;The geometric effects of VFe2+ for VMg substitution on the crystal structures
 of the grandidierite-ominelite series Sample: G2 Locality: Andrahomana,
 Madagascar
;
_journal_name_full               'American Mineralogist'
_journal_page_first              863
_journal_page_last               872
_journal_paper_doi               10.2138/am.2007.2275
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        'Andrahomana, Madagascar'
_chemical_formula_sum            'Al3 B Fe0.45 Mg0.55 O9 Si'
_chemical_name_mineral           Grandidierite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.3403
_cell_length_b                   11.0332
_cell_formula_units_Z            4
_cell_length_c                   5.7655
_cell_volume                     657.766
_database_code_amcsd             0004353
_exptl_crystal_density_diffrn    3.053
_cod_original_formula_sum        '(Mg.55 Fe.45) Al3 B Si O9'
_cod_database_code               9010232
The geometric effects of VFe2+ for VMg substitution on the crystal structures of the grandidierite-ominelite series Sample: G9 Locality: Almgjotheii, Rogaland, Norway
Dzikowski, T. J.; Groat, L. A.; Grew, E. S.; American Mineralogist 92 (2007) 863–872; doi:10.2138/am.2007.2275

data_9010233
_publ_section_title
;The geometric effects of VFe2+ for VMg substitution on the crystal structures
 of the grandidierite-ominelite series Sample: G9 Locality: Almgjotheii,
 Rogaland, Norway
;
_journal_name_full               'American Mineralogist'
_journal_page_first              863
_journal_page_last               872
_journal_paper_doi               10.2138/am.2007.2275
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        'Almgjotheii, Rogaland, Norway'
_chemical_formula_sum            'Al3 B Fe0.522 Mg0.478 O9 Si'
_chemical_name_mineral           Ominelite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.3450
_cell_length_b                   11.0519
_cell_formula_units_Z            4
_cell_length_c                   5.7656
_cell_volume                     659.192
_database_code_amcsd             0004354
_exptl_crystal_density_diffrn    3.069
_cod_original_formula_sum        '(Mg.478 Fe.522) Al3 B Si O9'
_cod_database_code               9010233
The geometric effects of VFe2+ for VMg substitution on the crystal structures of the grandidierite-ominelite series Sample: ominelite
Dzikowski, T. J.; Groat, L. A.; Grew, E. S.; American Mineralogist 92 (2007) 863–872; doi:10.2138/am.2007.2275

data_9010234
_publ_section_title
;The geometric effects of VFe2+ for VMg substitution on the crystal structures
 of the grandidierite-ominelite series Sample: ominelite
;
_journal_name_full               'American Mineralogist'
_journal_page_first              863
_journal_page_last               872
_journal_paper_doi               10.2138/am.2007.2275
_journal_volume                  92
_journal_year                    2007
_chemical_formula_sum            'Al3 B Fe O9 Si'
_chemical_name_mineral           Ominelite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.363
_cell_length_b                   11.129
_cell_length_c                   5.769
_cell_volume                     665.338
_cell_formula_units_Z            4
_database_code_amcsd             0004355
_exptl_crystal_density_diffrn    3.191
_cod_original_formula_sum        'Fe Al3 B Si O9'
_cod_database_code               9010234
Gram-Charlier development of the atomic displacement factors into mineral structures: The case of samsonite, Ag4MnSb2S6 Sample: T = 100 K
Bindi, L.; Evain, M.; American Mineralogist 92 (2007) 886–891; doi:10.2138/am.2007.2364

data_9010235
_publ_section_title
;
 Gram-Charlier development of the atomic displacement factors into mineral
 structures: The case of samsonite, Ag4MnSb2S6
 Sample: T = 100 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              886
_journal_page_last               891
_journal_paper_doi               10.2138/am.2007.2364
_journal_volume                  92
_journal_year                    2007
_chemical_compound_source        'St. Andreasberg, Hartz Mountains, Germany'
_chemical_formula_sum            'Ag4 Mn S6 Sb2'
_chemical_name_mineral           Samsonite
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 92.676
_cell_angle_gamma                90
_cell_length_a                   10.3702
_cell_length_b                   8.0647
_cell_length_c                   6.6400
_cell_formula_units_Z            2
_cell_volume                     554.715
_database_code_amcsd             0004356
_diffrn_ambient_temperature      100
_exptl_crystal_density_diffrn    5.522
_cod_original_formula_sum        'Ag4 Mn Sb2 S6'
_cod_database_code               9010235